SYNTHESIS AND CHARACTERIZATION OF NANOCRYSTALLINE properties of metals and ceramics. Therefore,...
Embed Size (px)
Transcript of SYNTHESIS AND CHARACTERIZATION OF NANOCRYSTALLINE properties of metals and ceramics. Therefore,...
SYNTHESIS AND CHARACTERIZATION OF NANOCRYSTALLINE CARBIDES BY REACTION MILLING
D. Chaira1, B.K. Mishra2ξ, S. Sangal3
1Department of Metallurgical & Materials Engineering, National Institute of Technology Rourkela, Orissa, India 2 CSIR-Institute of Minerals and Materials Technology, Bhubaneswar, Orissa, India
3Department of Materials & Metallurgical Engineering, Indian Institute of Technology Kanpur, U.P, India
Keywords: Dual drive planetary mill; Nanocrystalline carbides; Cementite; Silicon carbide; Titanium carbide; Reaction milling
ξ email : firstname.lastname@example.org
Abstract Nanocrystalline cementite, silicon carbide and titanium carbide powders were prepared from elemental constituent powder particles by reaction milling. A high energy dual drive planetary mill has been fabricated for the synthesis of carbides. The strong collision energy field of the dual drive planetary mill reduced the carbide formation time as compared to earlier reported studies. Forty hours is required to produce nanocrystalline cementite and silicon carbide powder. Whereas only 10 hours is required to produce titanium carbide powder, because self propagating reaction takes place between Ti and graphite during milling. The morphology of powders and evolution of different phases were studied by X-ray diffraction (XRD), scanning electron microscopy (SEM) and transmission electron microscopy (TEM).
Introduction Carbides possess unusual properties that make them desirable and useful engineering materials for many industrial applications. One important property of the carbides is their chemical stability at room temperature—they degrade slowly when subjected to highly concentrated acidic media. In fact, carbides are unique in that they combine the characteristic properties of metals and ceramics. Therefore, these materials are hard; resist wear; possess good thermal conductivity and oxidation resistance. For these reasons, carbides are used in a wide range of applications from refractory bricks to cutting tools. A systematic investigation is made with respect to the preparation in bulk and characterization of carbides. Three industrially important carbides viz., cementite (Fe3C), silicon carbide (SiC) and titanium carbide (TiC) are studied. These are synthesized up to 1 kg in batch from their corresponding elemental constituents by reaction milling in a specially built dual drive planetary mill. Cementite is a major constituent of iron-carbon alloys. These alloys attracted attention due to their low cost and high strength applications. Up until now, the interest in fabrication of Fe-C alloy had been focused only on low carbon concentration whereas high carbon concentrations were treated only on a limited scale. The main reason is that even today issues relating to interaction between different phases, effect of alloying element, etc., are not resolved, e.g. cementite is one of the most important phases in steel, which is responsible to a large extent
for its mechanical property. It also holds a lot of promise as a dispersoid for the synthesis of composites. The understanding of mechanical and physical properties of steel vis-à-vis cementite is not well established. Since cementite is hard and brittle at room temperature and meta-stable at all temperatures, it is difficult to synthesize and isolate as single-phase material under ordinary processing conditions. Cementite has no direct industrial application but it draws a lot of theoretical interest, as it is mainly responsible for the mechanical property of steel. Unlike cementite, silicon carbide (SiC) has many direct industrial applications. It is used in electronic devices that are particularly used at high temperatures. This is due to its high temperature electrical properties, high breakdown voltage and high electron mobility. It is also used in various types of high temperature applications such as heating elements and refractory material for furnaces due to its high fracture strength, excellent wear and creep resistance, high resistance to corrosion, good thermal conductivity and relatively low coefficient of thermal expansion. It is also a good filler material due to its thermal and chemical stability. This is valid both during synthesis and under severe service conditions. Titanium carbide (TiC) is a material of commercial interest because it possesses a number of desirable properties. It is one of the hardest known metal carbides (Ye, L. L. et al., 1995) and it exhibits excellent thermal stability and has a very high melting temperature of approximately 3100°C. It also displays relatively high thermal and electrical conductivity. In high temperature applications, higher thermal conductivity of TiC is an advantage as it results in lower thermal gradients, which reduces thermal stresses and cracking that makes it suitable for high-speed cutting tool applications. Similarly, good electrical conductivity of TiC makes it suitable for electrical discharge machining. Additionally, TiC has a low density, which is desirable for lightweight applications. It also exhibits excellent chemical stability, which is important for cutting tool applications, as chemical stability reduces the chemical interaction between the cutting tool and the work piece. The main aim of this work is to gain a better understanding of the reaction milling process and its products—Fe3C, SiC and TiC. The results of this work shall add to the fundamental understanding of the reaction milling process to synthesize carbides, which in turn can be utilized to pilot the process as a commercial option for bulk synthesis of carbides.
Frontiers in Mechanochemistry and Mechanical Alloying © CSIR-National Metallurgical Laboratory, Jamshedpur-831007, India, 2011
INCOME2008 1-4 December, 2008
Experimental Mill Design The dual drive planetary mill developed specifically for the synthesis of nanocrystalline carbides has a rotating shaft that sweeps a circle of diameter 750 mm. The two steel jars of 135 mm diameter (2500 ml each) rotate about their own axes around the common axis of the main shaft. The planetary mill is powered by two motors. A 5 HP motor works on the main rotating shaft and 3 HP motor drives the jars. The rotating speed of both motors can be varied independently and continuously by a frequency controller. This mill design follows closely the patented design of Rajamani et al. (2000) with several minor modifications to improve its performance and suit to the local conditions. Details of mill design and mill mechanics are available (Chaira et al. 2007). Figure 1 shows the dual drive planetary mill.
Figure 1. Dual drive planetary mill
Synthesis of Nanocrystalline Cementite Powder For the synthesis of cementite powder, iron and graphite powder with 99% purity were used in stoichiomatric ratio. Milling experiments were conducted in two jars each containing 250 grams of powder and 2.5 kg of steel balls for times varying from 6 hours to 50 hours. Sample of milled product was characterized by using X-ray diffraction, SEM and TEM.
Synthesis of Nanocrystalline Silicon Carbide Powder Silicon and graphite powder with 99.5 and 99% purity were taken as starting materials. Powders were mixed in 1:1 atomic ratio and milling was carried out for 40-hours in two jars-each containing 125 gm powder and 2.5 kg steel balls. Steel balls of diameter 6 and 12 mm were used for milling to study the effect of ball size. Synthesis of Nanocrystalline Titanium Carbide Powder In one jar titanium and graphite and in the other jar titanium and activated carbon were taken for the synthesis of TiC powder. Powders were taken in 1:1 atomic ratio. Here only 50 gm powder and 1 kg steel balls were taken for grinding. Milling was carried out for a period of 10 hours.
Results and Discussions Characterization of Cementite Powder In order to determine the phase change of the particle mixtures during the reaction milling process, a small sample of milled product was collected at regular intervals for X-ray diffraction analysis. The XRD patterns of the end product (as-milled powder) are shown in Fig. 2 for different intervals of milling time.
Figure 2. XRD patterns of Fe-6.7 wt% graphite powder at
selected milling times
Several interesting observations could be made from Fig. 2. First, the graphite peak disappeared after about 20 hours of milling. This is a general observation in this study, which may be due to amorphization of graphite during milling. Second, it was observed that the peak positions of iron shift to a lower angle with increasing milling time. The shift of the iron peaks position to the lower angle means that carbon atoms form a solid solution with iron. It was also observed that iron peaks broaden and their integrated intensity decreases with milling time. This suggests the accumulation of lattice strain and reduction of crystal size. Finally, peak corresponding to cementite is observed along with elemental iron and ferrite after 40-hours of grinding. Milling experiments beyond 40 hours were also done. However, no change in the intensity of the carbide peaks was
observed. Therefore, it is concluded that 40 hours was the optimum milling time. In comparison, Umemoto et al. (2004) produced bulk cementite from elemental iron and graphite powder by mechanical alloying in horizontal ball mill after 100 hours of milling. Wang and Campbell et al. (1995) also milled iron and graphite powder mixture in argon atmosphere